#------------------------------------------------------------------------------
#$Date: 2016-02-21 02:03:34 +0200 (Sun, 21 Feb 2016) $
#$Revision: 176798 $
#$URL: svn://www.crystallography.net/cod/cif/2/23/86/2238670.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2238670
loop_
_publ_author_name
'Salloum, Diala'
'Gougeon, Patrick'
'Gall, Philippe'
_publ_section_title
;
 Na~3.88~Mo₁₅Se₁₉: a novel ternary reduced molybdenum selenide
 containing Mo₆ and Mo₉ clusters
;
_journal_coeditor_code           RU2054
_journal_issue                   10
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i67
_journal_page_last               i68
_journal_paper_doi               10.1107/S1600536813025907
_journal_volume                  69
_journal_year                    2013
_chemical_formula_iupac          'Na3.88 Mo15 Se19'
_chemical_formula_moiety         'Mo15 Na3.88 Se19'
_chemical_formula_sum            'Mo15 Na3.88 Se19'
_chemical_formula_weight         3028.54
_chemical_name_systematic
;
Tetrasodium pentadecamolybdenum nonadecaselenide
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   9.86470(10)
_cell_length_b                   9.86470(10)
_cell_length_c                   19.5957(3)
_cell_measurement_reflns_used    26001
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      35.00
_cell_measurement_theta_min      1.70
_cell_volume                     1651.43(3)
_computing_cell_refinement       'COLLECT (Nonius, 1998)'
_computing_data_collection       'COLLECT (Nonius, 1998)'
_computing_data_reduction        'EvalCCD (Duisenberg, 1998)'
_computing_molecular_graphics    'DIAMOND (Bergerhoff, 1996)'
_computing_publication_material
'SHELXL97 (Sheldrick, 2008) and PLATON (Spek, 2009)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR97 (Altomare et al., 1999)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Nonius KappaCCD'
_diffrn_measurement_method       'φ scans (κ = 0) + additional ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0746
_diffrn_reflns_av_sigmaI/netI    0.0355
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            25999
_diffrn_reflns_theta_full        34.99
_diffrn_reflns_theta_max         34.99
_diffrn_reflns_theta_min         2.38
_exptl_absorpt_coefficient_mu    26.467
_exptl_absorpt_correction_T_max  0.2148
_exptl_absorpt_correction_T_min  0.1110
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
(de Meulenaer & Tompa, 1965)
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.091
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'multi-faceted crystal'
_exptl_crystal_F_000             2637
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.069
_exptl_crystal_size_min          0.059
_refine_diff_density_max         2.691
_refine_diff_density_min         -1.807
_refine_ls_extinction_coef       0.00058(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.056
_refine_ls_matrix_type           full
_refine_ls_number_parameters     67
_refine_ls_number_reflns         2487
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.056
_refine_ls_R_factor_all          0.0427
_refine_ls_R_factor_gt           0.0326
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0435P)²+3.7236P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0787
_refine_ls_wR_factor_ref         0.0836
_reflns_number_gt                2116
_reflns_number_total             2487
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ru2054.cif
_cod_data_source_block           I
_cod_original_sg_symbol_H-M      P63/m
_cod_database_code               2238670
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-y, x-y, z'
'-x+y, -x, z'
'x-y, x, z+1/2'
'y, -x+y, z+1/2'
'-x, -y, -z'
'x, y, -z-1/2'
'y, -x+y, -z'
'x-y, x, -z'
'-x+y, -x, -z-1/2'
'-y, x-y, -z-1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_symmetry_multiplicity
Mo Mo1 0.84973(5) -0.16457(5) 0.556745(19) 0.01378(9) Uani d . 1 1
Mo Mo2 0.68549(6) 0.18962(5) 0.63450(2) 0.01510(9) Uani d . 1 1
Mo Mo3 0.51739(7) 0.16952(8) 0.7500 0.01574(11) Uani d S 1 2
Se Se1 0.68259(6) -0.03045(6) 0.55145(2) 0.01653(11) Uani d . 1 1
Se Se2 0.38303(7) 0.00893(7) 0.63968(2) 0.01760(11) Uani d . 1 1
Se Se3 0.69343(10) 0.04771(10) 0.7500 0.01993(16) Uani d S 1 2
Se Se4 0.0000 0.0000 0.65840(4) 0.0222(2) Uani d S 1 3
Se Se5 0.6667 0.3333 0.53176(4) 0.01851(18) Uani d S 1 3
Na Na1 0.6667 0.3333 0.3864(3) 0.0618(18) Uani d S 1 3
Na Na2 0.0558(6) 0.2330(7) 0.7500 0.0214(16) Uani d SP 0.628(14) 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
Se4 Mo1 Se1 1_655 10_546 176.02(2)
Se4 Mo1 Se1 1_655 . 91.274(18)
Se1 Mo1 Se1 10_546 . 89.153(17)
Se4 Mo1 Se1 1_655 3_645 90.664(18)
Se1 Mo1 Se1 10_546 3_645 88.572(18)
Se1 Mo1 Se1 . 3_645 174.67(3)
Se4 Mo1 Mo1 1_655 3_645 57.759(12)
Se1 Mo1 Mo1 10_546 3_645 118.706(18)
Se1 Mo1 Mo1 . 3_645 119.10(2)
Se1 Mo1 Mo1 3_645 3_645 58.19(2)
Se4 Mo1 Mo1 1_655 4_765 57.759(12)
Se1 Mo1 Mo1 10_546 4_765 119.357(19)
Se1 Mo1 Mo1 . 4_765 59.15(2)
Se1 Mo1 Mo1 3_645 4_765 118.14(2)
Mo1 Mo1 Mo1 3_645 4_765 60.0
Se4 Mo1 Mo1 1_655 10_546 117.937(16)
Se1 Mo1 Mo1 10_546 10_546 58.50(2)
Se1 Mo1 Mo1 . 10_546 117.326(19)
Se1 Mo1 Mo1 3_645 10_546 57.453(14)
Mo1 Mo1 Mo1 3_645 10_546 60.209(10)
Mo1 Mo1 Mo1 4_765 10_546 90.0
Se4 Mo1 Mo1 1_655 9_666 117.937(16)
Se1 Mo1 Mo1 10_546 9_666 59.16(2)
Se1 Mo1 Mo1 . 9_666 57.743(15)
Se1 Mo1 Mo1 3_645 9_666 117.026(19)
Mo1 Mo1 Mo1 3_645 9_666 90.0
Mo1 Mo1 Mo1 4_765 9_666 60.209(9)
Mo1 Mo1 Mo1 10_546 9_666 59.583(19)
Se4 Mo1 Se2 1_655 4_655 91.21(2)
Se1 Mo1 Se2 10_546 4_655 92.77(2)
Se1 Mo1 Se2 . 4_655 87.51(2)
Se1 Mo1 Se2 3_645 4_655 97.41(2)
Mo1 Mo1 Se2 3_645 4_655 136.97(2)
Mo1 Mo1 Se2 4_765 4_655 130.63(2)
Mo1 Mo1 Se2 10_546 4_655 139.27(2)
Mo1 Mo1 Se2 9_666 4_655 132.73(2)
Se4 Mo1 Mo2 1_655 3_645 91.163(16)
Se1 Mo1 Mo2 10_546 3_645 91.320(19)
Se1 Mo1 Mo2 . 3_645 135.27(2)
Se1 Mo1 Mo2 3_645 3_645 49.629(15)
Mo1 Mo1 Mo2 3_645 3_645 99.53(2)
Mo1 Mo1 Mo2 4_765 3_645 148.233(15)
Mo1 Mo1 Mo2 10_546 3_645 100.519(16)
Mo1 Mo1 Mo2 9_666 3_645 149.644(19)
Se2 Mo1 Mo2 4_655 3_645 47.784(15)
Se4 Mo1 Mo1 1_655 7_756 87.495(19)
Se1 Mo1 Mo1 10_546 7_756 88.562(18)
Se1 Mo1 Mo1 . 7_756 87.95(2)
Se1 Mo1 Mo1 3_645 7_756 87.18(2)
Mo1 Mo1 Mo1 3_645 7_756 45.181(8)
Mo1 Mo1 Mo1 4_765 7_756 45.181(8)
Mo1 Mo1 Mo1 10_546 7_756 44.819(8)
Mo1 Mo1 Mo1 9_666 7_756 44.819(8)
Se2 Mo1 Mo1 4_655 7_756 175.25(3)
Mo2 Mo1 Mo1 3_645 7_756 136.78(2)
Se4 Mo1 Na2 1_655 3_655 45.18(9)
Se1 Mo1 Na2 10_546 3_655 138.79(9)
Se1 Mo1 Na2 . 3_655 82.95(8)
Se1 Mo1 Na2 3_645 3_655 101.91(8)
Mo1 Mo1 Na2 3_645 3_655 100.18(9)
Mo1 Mo1 Na2 4_765 3_655 90.73(8)
Mo1 Mo1 Na2 10_546 3_655 156.33(8)
Mo1 Mo1 Na2 9_666 3_655 138.84(7)
Se2 Mo1 Na2 4_655 3_655 46.69(8)
Mo2 Mo1 Na2 3_645 3_655 67.91(7)
Mo1 Mo1 Na2 7_756 3_655 131.19(9)
Se5 Mo2 Se2 . . 91.991(19)
Se5 Mo2 Mo2 . 4_665 58.558(12)
Se2 Mo2 Mo2 . 4_665 60.37(3)
Se5 Mo2 Mo2 . 3_655 58.558(12)
Se2 Mo2 Mo2 . 3_655 120.31(3)
Mo2 Mo2 Mo2 4_665 3_655 60.0
Se5 Mo2 Se2 . 3_655 91.314(18)
Se2 Mo2 Se2 . 3_655 175.53(3)
Mo2 Mo2 Se2 4_665 3_655 119.22(2)
Mo2 Mo2 Se2 3_655 3_655 59.27(2)
Se5 Mo2 Se3 . . 175.05(3)
Se2 Mo2 Se3 . . 86.12(2)
Mo2 Mo2 Se3 4_665 . 116.64(2)
Mo2 Mo2 Se3 3_655 . 118.69(2)
Se2 Mo2 Se3 3_655 . 90.35(3)
Se5 Mo2 Se1 . . 89.81(2)
Se2 Mo2 Se1 . . 85.71(2)
Mo2 Mo2 Se1 4_665 . 129.77(2)
Mo2 Mo2 Se1 3_655 . 137.17(2)
Se2 Mo2 Se1 3_655 . 97.31(2)
Se3 Mo2 Se1 . . 94.60(2)
Se5 Mo2 Mo3 . 3_655 120.52(2)
Se2 Mo2 Mo3 . 3_655 117.08(2)
Mo2 Mo2 Mo3 4_665 3_655 90.964(15)
Mo2 Mo2 Mo3 3_655 3_655 61.980(17)
Se2 Mo2 Mo3 3_655 3_655 58.547(18)
Se3 Mo2 Mo3 . 3_655 56.80(2)
Se1 Mo2 Mo3 . 3_655 139.02(2)
Se5 Mo2 Mo3 . . 119.05(2)
Se2 Mo2 Mo3 . . 58.376(18)
Mo2 Mo2 Mo3 4_665 . 60.511(18)
Mo2 Mo2 Mo3 3_655 . 90.119(16)
Se2 Mo2 Mo3 3_655 . 117.29(2)
Se3 Mo2 Mo3 . . 56.13(2)
Se1 Mo2 Mo3 . . 132.31(2)
Mo3 Mo2 Mo3 3_655 . 58.76(2)
Se5 Mo2 Mo1 . 4_765 91.085(16)
Se2 Mo2 Mo1 . 4_765 132.93(2)
Mo2 Mo2 Mo1 4_665 4_765 149.106(14)
Mo2 Mo2 Mo1 3_655 4_765 100.94(2)
Se2 Mo2 Mo1 3_655 4_765 49.978(15)
Se3 Mo2 Mo1 . 4_765 93.55(2)
Se1 Mo2 Mo1 . 4_765 47.329(15)
Mo3 Mo2 Mo1 3_655 4_765 101.18(2)
Mo3 Mo2 Mo1 . 4_765 149.02(2)
Se3 Mo3 Se3 . 4_665 176.87(3)
Se3 Mo3 Se2 . . 88.45(2)
Se3 Mo3 Se2 4_665 . 93.31(2)
Se3 Mo3 Se2 . 8_557 88.45(2)
Se3 Mo3 Se2 4_665 8_557 93.31(2)
Se2 Mo3 Se2 . 8_557 111.50(3)
Se3 Mo3 Mo3 . 3_655 58.60(4)
Se3 Mo3 Mo3 4_665 3_655 118.27(4)
Se2 Mo3 Mo3 . 3_655 117.76(2)
Se2 Mo3 Mo3 8_557 3_655 117.76(2)
Se3 Mo3 Mo3 . 4_665 118.60(3)
Se3 Mo3 Mo3 4_665 4_665 58.27(4)
Se2 Mo3 Mo3 . 4_665 120.43(2)
Se2 Mo3 Mo3 8_557 4_665 120.43(2)
Mo3 Mo3 Mo3 3_655 4_665 60.0
Se3 Mo3 Mo2 . 11_667 118.045(18)
Se3 Mo3 Mo2 4_665 11_667 60.968(17)
Se2 Mo3 Mo2 . 11_667 149.86(3)
Se2 Mo3 Mo2 8_557 11_667 59.121(17)
Mo3 Mo3 Mo2 3_655 11_667 89.853(16)
Mo3 Mo3 Mo2 4_665 11_667 61.335(19)
Se3 Mo3 Mo2 . 4_665 118.045(18)
Se3 Mo3 Mo2 4_665 4_665 60.968(17)
Se2 Mo3 Mo2 . 4_665 59.121(17)
Se2 Mo3 Mo2 8_557 4_665 149.86(3)
Mo3 Mo3 Mo2 3_655 4_665 89.853(16)
Mo3 Mo3 Mo2 4_665 4_665 61.335(19)
Mo2 Mo3 Mo2 11_667 4_665 112.93(3)
Se3 Mo3 Mo2 . 8_557 60.536(17)
Se3 Mo3 Mo2 4_665 8_557 118.389(19)
Se2 Mo3 Mo2 . 8_557 145.85(3)
Se2 Mo3 Mo2 8_557 8_557 57.914(17)
Mo3 Mo3 Mo2 3_655 8_557 59.903(18)
Mo3 Mo3 Mo2 4_665 8_557 89.039(15)
Mo2 Mo3 Mo2 11_667 8_557 57.509(17)
Mo2 Mo3 Mo2 4_665 8_557 146.42(3)
Se3 Mo3 Mo2 . . 60.536(17)
Se3 Mo3 Mo2 4_665 . 118.388(19)
Se2 Mo3 Mo2 . . 57.913(17)
Se2 Mo3 Mo2 8_557 . 145.85(3)
Mo3 Mo3 Mo2 3_655 . 59.903(18)
Mo3 Mo3 Mo2 4_665 . 89.039(15)
Mo2 Mo3 Mo2 11_667 . 146.42(3)
Mo2 Mo3 Mo2 4_665 . 57.508(17)
Mo2 Mo3 Mo2 8_557 . 110.55(3)
Se3 Mo3 Na2 . 4 115.38(12)
Se3 Mo3 Na2 4_665 4 67.75(12)
Se2 Mo3 Na2 . 4 60.24(4)
Se2 Mo3 Na2 8_557 4 60.24(4)
Mo3 Mo3 Na2 3_655 4 173.98(12)
Mo3 Mo3 Na2 4_665 4 126.02(12)
Mo2 Mo3 Na2 11_667 4 93.47(6)
Mo2 Mo3 Na2 4_665 4 93.47(6)
Mo2 Mo3 Na2 8_557 4 118.06(4)
Mo2 Mo3 Na2 . 4 118.06(4)
Mo1 Se1 Mo1 9_666 . 63.76(2)
Mo1 Se1 Mo1 9_666 4_765 63.39(2)
Mo1 Se1 Mo1 . 4_765 62.66(2)
Mo1 Se1 Mo2 9_666 . 132.81(3)
Mo1 Se1 Mo2 . . 129.41(2)
Mo1 Se1 Mo2 4_765 . 83.04(2)
Mo1 Se1 Na1 9_666 7_656 130.23(8)
Mo1 Se1 Na1 . 7_656 99.13(2)
Mo1 Se1 Na1 4_765 7_656 151.91(7)
Mo2 Se1 Na1 . 7_656 95.04(6)
Mo2 Se2 Mo3 . . 63.71(2)
Mo2 Se2 Mo2 . 4_665 60.36(2)
Mo3 Se2 Mo2 . 4_665 62.333(19)
Mo2 Se2 Mo1 . 3_545 127.69(2)
Mo3 Se2 Mo1 . 3_545 130.42(3)
Mo2 Se2 Mo1 4_665 3_545 82.24(2)
Mo2 Se2 Na2 . 4 129.48(9)
Mo3 Se2 Na2 . 4 65.90(8)
Mo2 Se2 Na2 4_665 4 98.77(11)
Mo1 Se2 Na2 3_545 4 88.56(10)
Mo2 Se2 Na1 . 7_656 103.57(2)
Mo3 Se2 Na1 . 7_656 122.35(10)
Mo2 Se2 Na1 4_665 7_656 160.83(7)
Mo1 Se2 Na1 3_545 7_656 102.71(7)
Na2 Se2 Na1 4 7_656 99.85(14)
Mo3 Se3 Mo3 . 3_655 63.13(3)
Mo3 Se3 Na2 . 3_655 157.67(13)
Mo3 Se3 Na2 3_655 3_655 139.20(13)
Mo3 Se3 Mo2 . 8_557 63.33(2)
Mo3 Se3 Mo2 3_655 8_557 62.236(19)
Na2 Se3 Mo2 3_655 8_557 121.81(2)
Mo3 Se3 Mo2 . . 63.33(2)
Mo3 Se3 Mo2 3_655 . 62.236(19)
Na2 Se3 Mo2 3_655 . 121.81(2)
Mo2 Se3 Mo2 8_557 . 115.04(3)
Mo3 Se3 Na2 . 1_655 125.24(11)
Mo3 Se3 Na2 3_655 1_655 62.11(11)
Na2 Se3 Na2 3_655 1_655 77.1(2)
Mo2 Se3 Na2 8_557 1_655 91.04(6)
Mo2 Se3 Na2 . 1_655 91.04(6)
Mo1 Se4 Mo1 1_455 3_545 64.48(2)
Mo1 Se4 Mo1 1_455 4_665 64.48(2)
Mo1 Se4 Mo1 3_545 4_665 64.48(2)
Mo1 Se4 Na2 1_455 4 127.86(10)
Mo1 Se4 Na2 3_545 4 94.05(8)
Mo1 Se4 Na2 4_665 4 149.31(10)
Mo1 Se4 Na2 1_455 . 149.31(9)
Mo1 Se4 Na2 3_545 . 127.86(10)
Mo1 Se4 Na2 4_665 . 94.05(8)
Na2 Se4 Na2 4 . 81.92(12)
Mo1 Se4 Na2 1_455 3 94.05(8)
Mo1 Se4 Na2 3_545 3 149.31(9)
Mo1 Se4 Na2 4_665 3 127.86(10)
Na2 Se4 Na2 4 3 81.92(12)
Na2 Se4 Na2 . 3 81.92(12)
Mo2 Se5 Mo2 3_655 . 62.88(2)
Mo2 Se5 Mo2 3_655 4_665 62.88(2)
Mo2 Se5 Mo2 . 4_665 62.88(2)
Mo2 Se5 Na1 3_655 . 142.963(15)
Mo2 Se5 Na1 . . 142.963(15)
Mo2 Se5 Na1 4_665 . 142.963(15)
Se5 Na1 Se2 . 7_656 99.20(10)
Se5 Na1 Se2 . 9_666 99.20(10)
Se2 Na1 Se2 7_656 9_666 117.49(6)
Se5 Na1 Se2 . 10_556 99.20(10)
Se2 Na1 Se2 7_656 10_556 117.49(6)
Se2 Na1 Se2 9_666 10_556 117.49(6)
Se5 Na1 Se1 . 9_666 69.42(9)
Se2 Na1 Se1 7_656 9_666 66.67(2)
Se2 Na1 Se1 9_666 9_666 65.44(2)
Se2 Na1 Se1 10_556 9_666 168.60(19)
Se5 Na1 Se1 . 7_656 69.42(9)
Se2 Na1 Se1 7_656 7_656 65.44(2)
Se2 Na1 Se1 9_666 7_656 168.60(19)
Se2 Na1 Se1 10_556 7_656 66.67(2)
Se1 Na1 Se1 9_666 7_656 108.34(9)
Se5 Na1 Se1 . 10_556 69.42(9)
Se2 Na1 Se1 7_656 10_556 168.60(19)
Se2 Na1 Se1 9_666 10_556 66.67(2)
Se2 Na1 Se1 10_556 10_556 65.44(2)
Se1 Na1 Se1 9_666 10_556 108.34(9)
Se1 Na1 Se1 7_656 10_556 108.34(9)
Se3 Na2 Se4 4_665 . 87.67(13)
Se3 Na2 Se4 4_665 8_557 87.67(13)
Se4 Na2 Se4 . 8_557 81.61(16)
Se3 Na2 Se2 4_665 12_557 111.08(14)
Se4 Na2 Se2 . 12_557 156.4(2)
Se4 Na2 Se2 8_557 12_557 84.93(4)
Se3 Na2 Se2 4_665 3 111.08(14)
Se4 Na2 Se2 . 3 84.93(4)
Se4 Na2 Se2 8_557 3 156.4(2)
Se2 Na2 Se2 12_557 3 100.51(17)
Se3 Na2 Mo3 4_665 3 146.9(2)
Se4 Na2 Mo3 . 3 116.51(14)
Se4 Na2 Mo3 8_557 3 116.51(14)
Se2 Na2 Mo3 12_557 3 53.86(9)
Se2 Na2 Mo3 3 3 53.86(9)
Se3 Na2 Se3 4_665 1_455 162.9(2)
Se4 Na2 Se3 . 1_455 79.44(13)
Se4 Na2 Se3 8_557 1_455 79.44(13)
Se2 Na2 Se3 12_557 1_455 79.14(11)
Se2 Na2 Se3 3 1_455 79.14(11)
Mo3 Na2 Se3 3 1_455 50.14(8)
Se3 Na2 Na2 4_665 3 116.92(17)
Se4 Na2 Na2 . 3 49.04(6)
Se4 Na2 Na2 8_557 3 49.04(6)
Se2 Na2 Na2 12_557 3 107.97(17)
Se2 Na2 Na2 3 3 107.97(17)
Mo3 Na2 Na2 3 3 96.1(2)
Se3 Na2 Na2 1_455 3 45.99(16)
Se3 Na2 Na2 4_665 4 56.92(17)
Se4 Na2 Na2 . 4 49.04(6)
Se4 Na2 Na2 8_557 4 49.04(6)
Se2 Na2 Na2 12_557 4 129.74(9)
Se2 Na2 Na2 3 4 129.74(9)
Mo3 Na2 Na2 3 4 156.1(2)
Se3 Na2 Na2 1_455 4 105.99(16)
Na2 Na2 Na2 3 4 60.0000(10)
Se3 Na2 Mo1 4_665 11_667 96.57(7)
Se4 Na2 Mo1 . 11_667 121.60(17)
Se4 Na2 Mo1 8_557 11_667 40.767(18)
Se2 Na2 Mo1 12_557 11_667 44.758(19)
Se2 Na2 Mo1 3 11_667 142.89(16)
Mo3 Na2 Mo1 3 11_667 89.52(8)
Se3 Na2 Mo1 1_455 11_667 80.99(8)
Na2 Na2 Mo1 3 11_667 78.76(9)
Na2 Na2 Mo1 4 11_667 85.87(7)
Se3 Na2 Mo1 4_665 4_665 96.57(7)
Se4 Na2 Mo1 . 4_665 40.767(18)
Se4 Na2 Mo1 8_557 4_665 121.60(17)
Se2 Na2 Mo1 12_557 4_665 142.89(16)
Se2 Na2 Mo1 3 4_665 44.758(19)
Mo3 Na2 Mo1 3 4_665 89.52(8)
Se3 Na2 Mo1 1_455 4_665 80.99(8)
Na2 Na2 Mo1 3 4_665 78.76(9)
Na2 Na2 Mo1 4 4_665 85.87(7)
Mo1 Na2 Mo1 11_667 4_665 157.26(17)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Mo1 Se4 1_655 2.5287(7) y
Mo1 Se1 10_546 2.5600(6) y
Mo1 Se1 . 2.5810(7) y
Mo1 Se1 3_645 2.6075(7) y
Mo1 Mo1 3_645 2.6980(7) y
Mo1 Mo1 4_765 2.6980(7) ?
Mo1 Mo1 10_546 2.7152(7) y
Mo1 Mo1 9_666 2.7152(7) ?
Mo1 Se2 4_655 2.7207(7) y
Mo1 Mo2 3_645 3.5202(6) ?
Mo1 Mo1 7_756 3.8278(8) ?
Mo1 Na2 3_655 3.8628(12) ?
Mo2 Se5 . 2.5220(7) y
Mo2 Se2 . 2.6023(8) y
Mo2 Mo2 4_665 2.6311(7) y
Mo2 Mo2 3_655 2.6311(7) ?
Mo2 Se2 3_655 2.6312(8) y
Mo2 Se3 . 2.6830(6) y
Mo2 Se1 . 2.7018(7) y
Mo2 Mo3 3_655 2.7153(6) y
Mo2 Mo3 . 2.7537(6) y
Mo2 Mo1 4_765 3.5202(6) ?
Mo3 Se3 . 2.5586(11) y
Mo3 Se3 4_665 2.5675(11) y
Mo3 Se2 . 2.6153(6) y
Mo3 Se2 8_557 2.6153(6) y
Mo3 Mo3 3_655 2.6834(11) y
Mo3 Mo3 4_665 2.6834(11) ?
Mo3 Mo2 11_667 2.7153(6) ?
Mo3 Mo2 4_665 2.7153(6) ?
Mo3 Mo2 8_557 2.7537(6) ?
Mo3 Na2 4 2.956(5) ?
Se1 Mo1 9_666 2.5600(6) ?
Se1 Mo1 4_765 2.6075(7) ?
Se1 Na1 7_656 3.462(2) ?
Se2 Mo2 4_665 2.6312(8) ?
Se2 Mo1 3_545 2.7207(7) ?
Se2 Na2 4 2.812(4) ?
Se2 Na1 7_656 3.2010(11) ?
Se3 Mo3 3_655 2.5675(11) ?
Se3 Na2 3_655 2.657(5) ?
Se3 Mo2 8_557 2.6830(6) ?
Se3 Na2 1_655 3.096(5) ?
Se4 Mo1 1_455 2.5287(7) ?
Se4 Mo1 3_545 2.5287(7) ?
Se4 Mo1 4_665 2.5287(7) ?
Se4 Na2 4 2.747(4) ?
Se4 Na2 . 2.747(4) ?
Se4 Na2 3 2.747(5) ?
Se5 Mo2 3_655 2.5220(7) ?
Se5 Mo2 4_665 2.5220(7) ?
Se5 Na1 . 2.848(6) y
Na1 Se2 7_656 3.2010(11) y
Na1 Se2 9_666 3.2010(11) ?
Na1 Se2 10_556 3.2010(11) ?
Na1 Se1 9_666 3.462(2) y
Na1 Se1 7_656 3.462(2) ?
Na1 Se1 10_556 3.462(2) ?
Na2 Se3 4_665 2.657(5) y
Na2 Se4 8_557 2.747(4) y
Na2 Se2 12_557 2.812(4) y
Na2 Se2 3 2.812(4) ?
Na2 Mo3 3 2.956(5) ?
Na2 Se3 1_455 3.096(5) y
Na2 Na2 3 3.601(10) ?
Na2 Na2 4 3.601(10) ?
Na2 Mo1 11_667 3.8628(12) ?
Na2 Mo1 4_665 3.8628(12) ?
